silver and/or copper vermiculites and their antibacterial effect
Acta Geodyn. Geomater., Vol. 10, No. 1 (169), 97–104, 2013
SILVER AND/OR COPPER VERMICULITES AND
THEIR ANTIBACTERIAL EFFECT
Marianna HUNDÁKOVÁ 1,2)*, Marta VALÁŠKOVÁ 1,2), Vladimír TOMÁŠEK 1),
Erich PAZDZIORA 3) and Kateřina MATĚJOVÁ 3)
Nanotechnology Centre, VŠB-Technical University of Ostrava, 17. listopadu 15, 708 33 Ostrava-Poruba,
IT4 Innovations Centre of Excellence, VŠB-Technical University of Ostrava, 17. listopadu 15,
708 33 Ostrava-Poruba, Czech Republic
National Reference Laboratory, Institute of Public Health in Ostrava, Partyzanske namesti 7,
702 00 Ostrava, Czech Republic
*Corresponding author‘s e-mail: [email protected]
(Received June 2012, accepted November 2012)
Vermiculite (V) from Brazil with aqueous solutions AgNO3 and/or Cu(NO3)2 was used for preparation of nanocomposites
V/Ag, V/Cu, V/AgCu and V/CuAg using two procedures and their effect on bacteria was compared. Structural changes were
evaluated using X-ray diffraction (XRD) analysis, Infrared spectroscopy (IRS) and Scanning electron microscopy (SEM).
Elemental chemical composition was determined using X-ray fluorescence (XRF) analysis and the solutions were analyzed by
Atomic emission spectroscopy with inductively coupled plasma (AES-ICP).
Antibacterial properties of Ag- and Cu-vermiculites and combined Ag/Cu-vermiculites were tested on two bacteria groups:
(1) Gram-positive, G+, (Staphylococcus aureus and Enterococcus faecalis) and (2) Gram-negative, G-, (Pseudomonas
aeruginosa and Klebsiella pneumoniae). The samples under antibacterial testing showed different effective times and
minimum inhibitory concentration (MIC) values. The Gram-negative bacteria showed higher sensitivity to the prepared
samples than Gram-positive bacteria. The combined Cu/Ag vermiculites stopped the bacterial growth at lower MIC value.
vermiculite; silver; copper; structure characterization; antibacterial effect
Clay mineral vermiculite belongs to a group of
planar hydrous phyllosilicates (layered silicates).
Vermiculite structure consists from an octahedral
sheet placed between two tetrahedral sheets which
together form a 2:1 layer. Between the layers is the
interlayer space containing hydrated exchangeable
cations as an interlayer material. The negative layer
charge of vermiculite 0.6 – 0.9 e- resulting from the
substitution of Al3+ for the tetrahedral central cation
Si4+ and Al3+ and/or Fe3+ for octahedral central cation
Mg2+ is balanced by exchangeable cations present in
the interlayer (Shirozu and Bailey, 1966; Bailey,
1980; Martin et al., 1991).
Clay minerals have many applications mainly in
ceramics as sorbents, catalysts or fillers in various
materials, though as well as a matrix for the
preparation of metal nanoparticles.
nanoparticles can be anchored on the external surface
of the clay mineral silicate layers or in their interlayer
The most common procedure employed for the
preparation of the metal nanoparticles is the reduction
from appropriate salts solutions. For example, silver
nanoparticles on montmorillonite substrates were
prepared using a silver nitrate solution in water
(Magaña et al., 2008; Valášková et al., 2007, 2010).
Other authors have described procedures, including an
additional step of silver nanoparticles’ preparation
with reducing agents such as sodium borohydride or
formaldehyde (Patakfalvi et al., 2003; Praus et al.,
2010, Miyoshi et al., 2010), ethylene glycol or
glycerol (Ayyppan et al., 1996; Valášková et al.,
2007), and also by using UV radiation (Huang and
Yang, 2008; Darroudi et al., 2009).
Copper bound on the clay minerals matrix as
a hydrate complex can be prepared by cation
exchange reaction (Morton et al., 2001; Strawn et al.,
2004; Furnare et al., 2005). Drelich et al. (2011)
prepared copper nanoparticles on the vermiculite
matrix from the cation exchanged Cu-form by
hydrogen reduction followed by heat treatment.
Silver and copper are known for their
antibacterial properties. Most of authors have studied
montmorillonite (Zhou et al., 2004; Hu et al., 2005;
Özdemir et al., 2010) and vermiculite (Li et al., 2002).
Cu-montmorillonites were studied in connection with
their potential utilization in veterinary medicine (Xia
et al., 2005; Hu and Xia, 2006; Tong et al., 2005; Yu
et al., 2008). The antibacterial influence of
Ag/montmorillonites and Ag/vermiculites was less
commonly studied (Magaña et al., 2008; Valášková et
al., 2010; Özdemir et al., 2010; Malachová et al.,
M. Hundáková et al.
2009). Özdemir et al. (2010) compared the
antibacterial effect of Ag-, Cu- and Zn- forms of
montmorillonite. The authors have found good
antibacterial effect of Cu- and Ag-montmorillonite
against bacterial strains Pseudomonas aeruginosa and
As described in the previous research works,
silver and copper were sporadically studied on the
vermiculite. Preparation of the combined content Ag
and Cu on the vermiculite matrix as well as study
of their antibacterial effect has not yet been
reported. The present work examines the structure
and antibacterial effect of Ag/Cu-vermiculites on
the bacteria strains: Gram-positive (Staphylococcus
aureus and Enterococcus faecalis) and Gram-negative
Vermiculite from Brazil was used as a starting
material. The particle size fraction < 40 μm was
obtained by milling in a planetary mill for 20 min
and sieving by a sieve with a pore size of less than
40 μm. The half unit cell composition of the
vermiculite sample (Si3.08Al0.92)(Mg2.44Fe 0.36 Fe 0.02
Ti0.06Al0.04)O10(OH)2 K0.18Ca0.15Na0.08 was calculated
from the results of elemental analysis. Silver nitrate,
AgNO3 and copper nitrate, Cu(NO3)2 (fy Mach chem.,
CZ) with the purity of 99.99 % were used as sources
of silver and copper.
2.2. SAMPLE PREPARATION
Four samples were prepared using two
procedures: P1, P2:
P1. Samples V/Ag and V/Cu were prepared from
vermiculite (V) and the 0.1 mol.dm-3 aqueous solution
AgNO3 and 0.1 mol.dm-3 Cu(NO3)2, respectively, at
the rate of 1:10 (grams of vermiculite : millilitre of
solution), and the suspension was shaken for 24 hours.
P2. Sample V/AgCu was prepared mixing the
sample V/Ag in the 0.1 mol.dm-3 aqueous solution
Cu(NO3)2. Similarly, the sample V/CuAg was
prepared from the sample V/Cu and the 0.1 mol.dm-3
aqueous solution AgNO3.
All prepared samples were centrifuged and
washed with distilled water until nitrate ions were not
present, and then dried at 70 °C for 24 h. The samples
with silver were protected before the light by
aluminium foil during the preparation.
X-ray powder diffraction
The X-ray powder diffraction (XRD) patterns
were measured on the X-ray diffractometer from
INEL equipped with a 120° curved position-sensitive
detector CPSD 120 (reflection mode, Gemonochromatized CuKα1 radiation). All patterns were
recorded at 30 kV and 20 mA, exposure time 2000 s,
with the samples in a flat rotation holder.
Scanning electron microscopy
Morphology and the surfaces of samples were
studied using Scanning electron microscopy (SEM) on
PHILIPS XL-30 equipped with energy dispersive
spectrometer (EDS) for elemental analysis and
Fourier transform infrared spectroscopy
The mid-infrared spectra were obtained by
Fourier transform infrared spectroscopy (FTIR) on
a Perkin Elmer 2000. The measurement was carried
out in the spectral range 4000-400 cm-1 with a resolution of 4 cm-1 at room temperature using the KBr
X-ray fluorescence analysis
The elemental composition of samples and the
content of silver and copper were determined by Xray fluorescence elemental analysis (XRF) on an
energy dispersive spectrometer SPECTRO X LAB
with Rh X-ray lamp and secondary and polarization
Atomic emission spectroscopy
Atomic emission spectroscopy with inductively
coupled plasma (AES-ICP) on a Jobin-Yvon JY-24
spectrometer was used for determination of elements
at leaches after modification.
2.4. ANTIBACTERIAL TEST
The antibacterial activity of the prepared
nanocomposites was examined using two different
groups of experimental bacterial strains. The Gramnegative
(G-) strain represented the bacteria
Klebsiella pneumoniae (K. pneumoniae, CCM 4415)
and Pseudomonas aeruginosa (P. aeruginosa,
CCM 1960). The Gram-positive (G+) bacterial strain
was studied on the bacteria Staphylococcus aureus
(S. aureus, CCM 3953) and Enterococcus faecalis
(E. faecalis, CCM 4224).
The broth dilution method (Kneiflová, 1988) was
used for determination of the minimum inhibitory
concentration of silver and/or copper (MICAg/Cu)
in samples as the lowest concentration of silver
and/or copper that completely inhibits bacterial
growth. The bacterial suspension was prepared by
a twenty-hour cultivation in glucose broth. The
density of the glucose suspension used for individual
bacteria was: S. aureus (1.0 109 cfu ml-1), E faecalis
(1.1 109 cfu ml-1), K. pneumoniae (1.2 109 cfu ml-1),
P. aeruginosa (1.1 109 cfu ml-1). The silver and
copper vermiculite samples were prepared for
testing as a 10 % water dispersion, which was further
diluted to 3.33 %, 1.11 %, 0.37 %, 0.12 % and
0.041 %. The detailed procedure of antibacterial test is
published in Valášková et al. (2010).
SILVER AND/OR COPPER VERMICULITES AND THEIR ANTIBACTERIAL EFFECT
Table 1 The content of silver and copper at
Table 2 Concentration of elements
leached from vermiculite.
V/Ag V/Cu V/AgCu
(mmol .g )
3. RESULTS AND DISCUSSION
3.1. QUANTITY OF SILVER AND COPPER AT
The quantity of silver and copper fixed in
vermiculite is given in Table1. Sample V/Ag and
V/Cu contained the highest content of Ag and Cu
(0.52 and 0.33 mmol.g-1, respectively). The content
of silver in sample V/Ag after the following treatment
with Cu(NO3)2 solution decreased from 0.52 to
0.15 mmol.g-1 in sample V/AgCu. Additional
treatment V/Cu with AgNO3 solution slightly
decreased the content of copper from 0.33 mmol.g-1 to
0.25 mmol.g-1 in sample V/CuAg. The content of
silver 0.52 mmol.g-1 in the sample V/Ag was reduced
to 0.33 mmol.g-1 in V/CuAg.
These quantity differences resulted from the
ways of binding silver and copper cations in
vermiculite, and the ability of cations to bind
molecules in the interlayer. It was described that (i)
the copper on the vermiculite substrate is
predominantly positioned in the interlayer where
cations are surrounded by water molecules, and also
can be adsorbed on hydroxyl edge sites (Clementz et
al., 1973; McBride, 1976; Morton et al., 2001) and
that (ii) the silver in the interlayer can be present in
the form Ag+ and also Ag0 without water molecules
and on the surface of vermiculite as the silver
nanoparticles (Magaňa et al., 2008; Valášková et al.,
2007; Tokarský et al., 2010a, 2010b).
The sample V/AgCu contained approximately
70 % lower content of silver than the original sample
V/Ag. The sample V/CuAg showed a decrease about
25 % of copper in comparison with the original
sample V/Cu. This observation confirmed that the
copper was more strongly anchored to vermiculite
3.2. CONTENT OF LEACHED ELEMENTS
The elements released from the vermiculite
structure in Table 2 showed the following results: The
content of Na+ leached from the natural vermiculite
was higher in the AgNO3 solution than in the
Cu(NO3)2 solutions. This finding confirmed cation
exchange of Na+ for Ag+ and is in agreement with
observations reported in literature (Rivera-Garza et
al., 2000; de la Rosa Gomez et al., 2008). Similarly,
the higher divalent Ca2+ exchanged for Cu2+ was
confirmed by higher content of Ca2+ determined after
treatment in the Cu(NO3)2 solution than in the AgNO3
solution. It was also observed that the solution
Cu(NO3)2 contributed to the release not only of
divalent cations Ca2+ and Mg2+ but also Si4+ from
3.3. X-RAY DIFFRACTION ANALYSIS
The XRD pattern of the original V (Fig. 1)
shows the intensive basal diffraction with d(001) =
1.42 nm. The interlayer space value corresponds to the
two-layer hydrate phase (Walker, 1956). The
other two low-intensive and broad diffractions with
d = 1.24 nm and d = 2.32 nm match the one-layer
hydrate domains and mix-layered water molecules
domains, respectively (Marcos et al., 2009).
Exfoliation of the layered vermiculite structure
resulted in a decrease in the intensities of the basal
diffractions. If we consider the observed integral
intensity of basal reflection (001) with d(001) =
1.42 nm for V as 100 % (relative intensity), we can
calculate the percentage decrease in the relative
intensity of (001) reflection to 73 % at V/Cu (Fig. 1b)
and to 9 % in V/Ag (Fig. 1e). The next broad
diffraction with d = 1.24 nm in V shifted to the
smaller interlayer space (e.g. to the d = 1.1 nm in
V/AgCu) and proved formation of mixtures of less
hydrated phases. The metal silver was observed only
on the XRD pattern of the sample V/Ag as low
intensive diffractions d(111) = 0.236 nm and d(200) =
0.204 nm (Fig. 1e).
3.4. INFRARED SPECTROSCOPY
The IR spectra of the samples in Figure 2
showed the shift of the stretching vibration of water
O-H groups at 3420 cm-1 in V to 3440 cm-1 in V/Ag
and to 3446 cm-1 in V/CuAg.
In the case of samples V/Cu, V/CuAg and
V/AgCu, this band at 3420 cm-1 became wide and the
new bands at 3527 cm-1 and 3549 cm-1 appeared, and
are probably associated with Cu-for-Mg substitution
(Farmer and Russell, 1964). The band 1646 cm-1
belongs to the deformation vibrations of the water OH groups. The shift of this band was, in sample
V/AgCu, to 1635 cm-1, contrary to the V/CuAg, where
the new band at 1541 cm–1 indicated different
coordinated water forms, probably owing to the type
of the interlayer cations (Madejová, 2003).
Accordingly, in our samples the wavenumbers shifts
M. Hundáková et al.
The XRD patterns of basal diffractions (from 2° to 10° 2θ) and Ag diffractions (from 35° to
50° 2θ) of V (a), V/Cu (b), V/CuAg (c), V/AgCu (d) and V/Ag (e).
depend on the type of predominant cation in the
interlayer. The band at 1002 cm-1 belongs to the
stretching vibrations of Si-O-Si. The band at 812 cm-1
was ascribed to the bending vibrations of hydroxyl
groups shared between Al3+ and Mg2+ ions (Farmer
and Russell, 1964); the band at 739 cm-1 are the
bending vibrations of tetrahedral Si-O. The position
shifted from 685 cm–1 at V to the slightly lower
vibrations 683 cm–1 at V/Cu, V/CuAg and V/AgCu
involves bending vibrations of Mg3OH and Mg2AlOH
(Farmer, 1974; Madejová, 2003). The band around
458 cm–1 was assigned to bending vibrations Si-O-M
(where M can be Si, Mg, Al or Fe) (Van der Marel
and Beutelspacher, 1976).
3.5. SCANNING ELECTRON MICROSCOPY
The images of the samples with the spot
elemental analysis are shown in Figures 3 and 4. The
characteristic lamellar morphology of vermiculite
was, after treatment, partially disturbed. The treatment
with Cu(NO3)2 solution caused the vermiculite flakes
change to the flocky aggregates (Fig. 3c).
3.6. ANTIBACTERIAL ACTIVITY
The samples under antibacterial test showed
different effective times and MICAg/Cu values
(Tables 3 and 4). The sample V/Ag had a positive
effect against the G- bacteria and stopped bacterial
growth after 24 h (MICAg = 0.21 mg.l-1). The sample
V/Cu also showed the positive effect for all bacteria
regarding MIC (MICCu = 0.69 mg.l-1) and short
effective time of 5 h to suspend bacterial growth.
The sample V/AgCu after 24 h showed the lowest
MIC from all of the samples on the G- bacteria
P. aeruginosa (MICAg/Cu = 0.06/0.07 mg.l-1). On the
other hand the V/CuAg was the most effective in
stopping bacterial grow of G+ bacteria - S. aureus
(MICAg/Cu = 0.13/0.06 mg.l-1) after 24 h.
The difference of activity of bacteria G+ and
G are caused by structural variations of their cell
walls. While the G- bacteria have an outer membrane
layer of cells formed by lipopolysacharides and
phospholipids, and only a thin layer of peptidoglycan,
the G+ bacteria cell is composed of many layers of
peptidoglycan and lipoteichoic acid. The G+ bacteria
cell is simpler and more resistant, probably thanks to
a rough layer of peptidoglycan.
Distinct action of Ag and Cu on bacteria was
ascribed to several mechanisms (Abad et al., 1994;
Tong et al., 2005). Both elements can be attached by
the negatively charged bacterial cell and disturb the
cell walls and permeability and react with sulphur-
SILVER AND/OR COPPER VERMICULITES AND THEIR ANTIBACTERIAL EFFECT
The infrared spectra from 4000 to 2600 cm-1 and from 1800 to 400 cm-1 of V (a),
V/Ag (b), V/AgCu (c), V/CuAg (d) and V/Cu (e).
and phosphorus- groups of enzymes, proteins and
DNA as well. These metals can also cause oxidative
stress by generation of hydroxide radicals (Samuni et
al., 1981; Thurman and Gerba, 1989). The increased
negative effect of combined Ag, Cu - vermiculites on
bacteria could be ascribed to their synergic effect on
bacteria (Lin et al., 1996).
In this study the antibacterial vermiculites with
Ag and/or Cu were prepared and characterized.
Vermiculite layered structure after treatment with
AgNO3 and/or Cu(NO3)2 became the mixtures of
differently hydrated layers domains.
The sample V/Ag showed the highest content of
Ag. Samples V/Cu and V/AgCu contained the highest
amount of Cu.
The natural vermiculite had no effect on bacteria growth. The Gram negative P. aeruginosa and
K. pneumoniae were more sensitive to sample V/Cu
than to the V/Ag, and the antibacterial effect was
observed after 5 h and 24 h, respectively. Combined
Cu/Ag vermiculites stopped the bacterial growth at
lower MIC values. The Gram negative P. aeruginosa
growth was inhibited after 24 h at the lowest
concentration of the sample V/AgCu when the MIC
of the Ag and Cu was 0.06 mg.l-1 and 0.07 mg.l-1,
respectively. The Gram positive bacteria S. aureus
was the most sensitive to the sample V/CuAg and
inhibited growth after 24h at the lowest MIC of Ag
and Cu of 0.13 mg.l-1 and 0.06 mg.l-1. Gram positive
E. faecalis stopped growth after 48 h action of sample
V/Cu (MIC of Cu 0.69 mg.l-1).
This work was supported by projects: Ministry
of education, Youth and Sport of Czech Republic
SP2012/43, the Czech Grant Agency GA ČR
P210/11/2215 and the IT4Innovations Centre of
Excellence project reg. no.cz.1.05/1.1.00/02.0070.
The authors thank to J. Seidlerová for ICP-AES
analysis, M. Heliová and S. Kozubová for SEM
images, S. Holešová for IR spectra and D. Casten for
linguistic correction of the text.
Abad, F.X., Pintó, R.M., Diez, J.M. and Bosch, A.: 1994,
Disinfection of human enteric viruses in water by
copper and silver in combination with low levels of
chlorine. Appl. Environ. Microbiol., 60, 2377– 2383.
Ayyappan, S., Subbanna, G.N., Gopalan, R.S. and Rao,
C.N.R.: 1996, Nanoparticles of nickel and silver
produced by the polyol reduction of the metal salts
intercalated in montmorillonite. Solid State Ionics,
Bailey, S.W.: 1980, Summary of recommendations of
AIPEA nomenclature committee on clay minerals.
Am. Mineral., 65, 1–7.
M. Hundáková et al.
SEM images of V (a), V/Ag (b) and V/Cu (c) and their spectrum of spot elemental analysis.
Table 3 The results of antibacterial test for the Gram-positive bacteria.
S. aureus (G+)
E. faecalis (G+)
SILVER AND/OR COPPER VERMICULITES AND THEIR ANTIBACTERIAL EFFECT
SEM images of V/AgCu (a) and V/CuAg (b) and their spectrum of spot elemental analysis.
Table 4 The results of antibacterial test for the Gram-negative bacteria.
P. aeruginosa (G-)
K. pneumoniae (G-)
Clementz, D.M., Pinnavaia, T.J. and Portland, M.M.: 1973,
Stereochemistry of hydrated copper (II) ions on the
interlamellar surfaces of layer silicates. An electron
spin resonance study. J. Phys. Chem., 77, 196–200.
Darroudi, M., Ahmad, M.B., Shameli, K., Abdullah, A.H.,
Ibrahim, N.A.: 2009, Synthesis and characterization of
UV-irradiated silver/montmorillonite nanocomposites.
Solid State Sci., 11, 1621–1624.
De la Rosa-Gomez, I., Olguına, M.T. and Alcantara, D.:
2008, Antibacterial behavior of silver-modified
clinoptilolite–heulandite rich tuff on coliform
microorganisms from wastewater in a column system.
J. Env. Man., 88, 853–863.
Drelich, J., Li, B., Bowen, P., Hwang, J.-Y., Mills, O. and
Hoffmann, D.: 2011, Vermiculite decorated with
copper nanoparticles: Novel antibacterial hybrid
material. A. Surf. Sci., 257, 9435–9443.
Farmer, V.C.: 1974, The Infrared Spectra of Minerals.
Monograph 4, Mineralogical Society, London.
Farmer, V.C. and Russell, J.D.: 1964, The infrared spectra
of layer silicates. Spectrochim. Acta, 20, 1149–1173.
Furnare, L.J., Vailionis, A. and Strawn, D.G.: 2005,
Molecular-level investigation into copper complexes
on vermiculite: Effect of reduction of structural iron
on copper complexation. J. Colloid. Interface Sci.,
M. Hundáková et al.
Hu, C.H. and Xia, M.S.: 2006, Adsorption and antibacterial
effect of copper-exchanged montmorillonite on
Escherichia coli K88. Appl. Clay Sci., 31, 180–184.
Hu, C.H., Xu, Z.R. and Xia, M.S.: 2005, Antibacterial effect
of Cu2+-exchanged montmorillonite on Aeromonas
hydrophila and discussion on its mechanism. Vet.
Microbiol., 109, 83–88.
Huang, H. and Yang, Y.: 2008, Preparation of silver
nanoparticles in inorganic clay suspensions. Compos.
Sci. Technol., 68, 2948–2953.
Kneiflová, J.: 1988, Evaluation of the antibacterial effect of
disinfectants using a suspension micro-method
(Hodnocení baktericidní účinnosti dezinfekčních
epidemiologie, mikrobiologie a imunologie, 37, 97–
104, (in Czech)..
Li, B., Yu, S., Hwang, J.Y. and Shi, S.: 2002, Antibacterial
vermiculite nano–material. J. Miner. Mater. Char.
Eng., 1, 61–68.
Lin, Y.E., Vidic, R.D., Stout, J.E. and Yu, V.L.: 1996,
Individual and combined effects of copper and silver
ions on inactivation of Legionella Pneumophila. Wat.
Res., 30, 1905–1913.
Madejová, J.: 2003, FTIR techniques in clay mineral
studies. Vib. Spectrosc., 31, 1–10.
Magaña, S.M., Quintana, P., Aquilatr, D.H., Toledo, J.A.,
Ángeles-Chávez, C., Cortés, M.A., León, L., FreilePelegrín, Y., Lopt, T. and Torres Sánchez, R.M.:
2008, Antibacterial activity of montmorillonites
modified with silver. J. Mol. Catal. A: Chem.,
Malachová, K., Praus, P., Pavlíčková, Z. and Turicová, M.:
immobilised on montmorillonite. Appl. Clay Sci.,
Marcos, C., Arango, Y.C. and Rodriguez, I.: 2009, X-ray
diffraction studies of the thermal behaviour of
commercial vermiculites. Appl. Clay Sci., 42, 368–
Martin, R.T., Bailey, S.W., Eberl, D.D., Fanning, D.S.,
Guggenheim, S., Kodama, H., Pevear, D.R., Šrodoň, J.
and Wicks, F.J.: 1991 Report of the clay minerals
classification of clay materials. Clays Clay Miner.,
McBride, M.: 1976, Hydration structure of exchangeable
Cu2+ in vermiculite and smectite. Clays Clay Min.,
24, 211– 212.
Miyoshi, H., Ohno, H., Sakai, K., Okamura, N. and Kourai,
H.: 2010, Characterization and photochemical and
antibacterial properties of highly stable silver
nanoparticles prepared on montmorillonite clay in nhexanol. J. Colloid. Interface Sci., 345, 433–441.
Morton, J.D., Semnu, J.D. and Hayes, K.F.: 2001, An X-ray
absorption spectroscopy study of the structure and
reversibility of copper adsorbed to montmorillonite
clay. Geochim. Cosmochim. Acta, 65, 2709–2722.
Özdemir, G., Limoncu, M.H. and Yapar, S.: 2010, The
antibacterial effect of heavy metal and cetylpridiniumexchanged montmorillonites. Appl. Clay Sci.,
Patakfalvi, R., Oszkó, A. and Dékány, I.: 2003, Synthesis
and characterization of silver nanoparticle/kaolinite
composites. Colloid. Surf. A: Physicochem. Eng.
Asp., 220, 45–54.
Praus, P., Turicová, M., Machovič, V., Študentová, S. and
Klementová, M.: 2010, Characterization of silver
nanoparticles deposited on montmorillonite. Appl.
Clay Sci., 49, 341–345.
Rivera-Garza, M., Olguín, M.T., García-Sosa, I., Alcántara,
D. and Rodríguez-Fuentes, G.: 2000, Silver supported
on natural Mexican zeolite as an antibacterial material,
Micropor. Mesopor. Mater., 39, 431–444.
Samuni, A., Chevion, M. and Czapski, G.: 1981, Unusual
copper-induced sensitization of the biological damage
due to superoxide radicals. J. Biol. Chem., 256,
Shirozu, H., Bailey, S.W.: 1966, Crystal structure of a twolayer Mg-vermiculite. Am. Mineral., 51, 1124-1143.
Strawn, D.G., Palmer, N.E., Furnare, L.J., Goodell, C.,
Amonite, J.E. and Kukkadapu, R.K.: 2004, Copper
sorption mechanisms on smectites. Clays Clay Miner.,
Thurman, R. and Gerba, C.: 1989, The molecular
mechanisms of copper and silver ion disinfection of
bakteria and viruses. Crit. Rev. Env. Contr., 18, 295–
Tokarský, J., Čapková, P., Klemm, V., Rafaja, D. and
Kukutschová, J.: 2010a, Adhesion of silver
nanoparticles on the montmorillonite surface. J. Phys.
Chem. Sol., 71, 634–637.
Tokarský, J., Čapková, P., Rafaja, D., Klemm, V.,
Valášková, M., Kukutschová, J. and Tomášek, V.:
2010b, Adhesion of silver nanoparticles on the clay
substrates; modeling and experiment. Appl. Surf. Sci.,
Tong, G., Yulong, M., Peng, G. and Zirong, X.: 2005,
Antibacterial effects of the Cu(II)-exchanged
montmorillonite on Escherichia coli K88 and
Salmonella choleraesuis. Vet. Microbiol., 105, 113–
Valášková, M., Hundáková, M., Mamulová Kutláková, K.,
Seidlerová, J., Čapková, P., Pazdziora, E., Matějová,
K., Heřmánek, M., Klemm, V. and Rafaja, D.: 2010,
Preparation and characterization of antibacterial
Geochim. Cosmochim. Acta, 74, 6287–6300.
Valášková, M., Simha Martynková, G., Lešková, J.,
Čapková, P., Klemm, V. and Rafaja, D.: 2007, Silver
nanoparticles/Montmorillonite composites prepared
using nitrating reagent at water and glycerol. J.
Nanosci. Nanotechnol., 8, 1–9.
Van der Marel, H.W. and Beutelspacher, H.: 1976, Atlas of
infrared spectroscopy of clay minerals and their
admixtures. Elsevier Scientific Publishing Company,
Walker, G. F.: 1956, Mechanism of dehydration of Mgvermiculite. Clays Clay Min., 4, 101–115.
Xia, M.S., Hu, C.H. and Xu, Z.R.: 2005, Effects of copper
bearing montmorillonite on the growth performance,
intestinal microflora and morphology of weanling
pigs. Anim. Feed Sci. Tech., 118, 307–317.
Yu, D.Y., Li, X.L. and Li, W.F.: 2008, Effect of
Montmorillonite Superfine Composite on Growth
Performance and Tissue Lead Level in Pigs. Biol.
Trace Elem. Res., 125, 229–235.
Zhou, Y., Xia, M., Ye, Y. and Hu, C.: 2004, Antimicrobial
ability of Cu2+-montmorillonite. Appl. Clay Sci.,
27, 215– 218.